Effects of addition of BaTiO3 Nano particles on the conductivity of PVdF/PMMA based polymer blend electrolytes
International Journal of Engineering Inventionse-ISSN: 2278-7461, p-ISSN: 2319-6491Volume 2, Issue 4 (February 2013) PP: 49-53www.iosrjournals.org 49 | PageEffects of addition of BaTiO3 Nano particles on the conductivityof PVdF/PMMA based polymer blend electrolytesM. Ramesh Prabhu*, S. RajendraSchool of Physics, Alagappa University, Karaikudi, 630 003, IndiaAbstract: Composite polymer electrolyte (CPE) membranes, comprising poly (vinylidene fluoride) (PVdF)/poly(methyl methacrylate) (PMMA), BaTiO3 as ceramic filler and LiBF4 as the lithium salt were prepared using asolution casting technique. The prepared membranes were subjected to XRD, FT-IR, impedance spectroscopyand thermal stability studies. The incorporation of nanofiller greatly enhanced the ionic conductivity and thethermal stability of the composite polymer electrolyte. Polymer blend electrolyte with 15 wt% of BaTiO3ceramic powder exhibited higher ionic conductivity (1.335 x 10-3S/cm) compared to the other ratios.Keywords: Polymer electrolyte; Composite; Inert filler; Plasticizer; Impedance studies.I. IntroductionIn recent years, there has been a growing demand for high-energy density rechargeable batteries forportable electronic products. The science of polymer electrolytes is a highly specialized interdisciplinary fieldwhich encompasses the disciplines of electrochemistry, polymer science, organic chemistry, and inorganicchemistry. The field has attracted ever-increasing interest both in academia and industry [1, 2]. Since Wright etal.  found out in 1973 that the complex of poly (ethylene oxide) (PEO) and alkaline salts have the ability ofionic conductivity. Solid polymer electrolytes (SPEs) have drawn significant interest for the possiblereplacement of liquid electrolytes in secondary lithium batteries due to the advantages of SPE-based lithiumbatteries considering safety, weight and size . The main reason in choosing these polymers the host is that itforms more stable complexes and possesses higher ionic conductivities than any other group of solvatingpolymers without the addition of organic solvents .Thus, several approaches have been applied to enhance the properties of polymer electrolytes. One ofthe most effective approaches has been the addition of inorganic fillers, such as ceramic fillers , as well assyntheses of organic/inorganic hybrid materials . The results showed that the addition of the inorganic fillershas improved many properties of the polymer electrolytes, such as ionic conductivity, lithium ion transferencenumber (t+), mechanical properties, and the stability of electrolyte–electrode interface . These improvementshave been ascribed to fillers that (1) acted as the plasticizers and lowered the crystallinity of the polymer matrix, (2) increased ion mobility by providing additional conductive pathway due to formation of the Lewis acid–base interactions , and (3) increased the number of charge carriers due to enhancement of the saltdissociation  .In this work, we investigated preparation of PVdF/PMMA based composite polymer blend electrolytescomposed of LiBF4 as a salt and BaTiO3 as a ceramic filler. This study focuses on improvement of the ionicconductivities of polymer electrolytes by the addition of BaTiO3 nanoparticles. The effects of the BaTiO3nanoparticles on the performance of polymer electrolytes are presented and discussed.II. Materials and MethodsPVdF and PMMA (both from Aldrich) were dried under vacuum at 80C for 24 hours. Reagent gradeanhydrous lithium tetraflouro borate was used after drying in vacuum at 110C for 24 hours. The plasticizerpropylene carbonate (PC) (from Aldrich) was used as supplied. The nano sized BaTiO3 (Aldrich) was used as aceramic filler. All the electrolytes have been prepared by the solvent casting technique. Appropriate quantities ofPVdF, PMMA and LiBF4 are dissolved by adding in sequence to tetrahydrofuran (THF) and stirred for 24h. Theresulting solution is poured on to a glass plate and the THF is allowed to evaporate in air at room temperaturefor several hours. The films are further dried at 60º C for 24 hours in vacuum to remove any traces of THF.Thin films thus obtained were subjected to XRD and FTIR studies to investigate the complexationbehaviour and the nature of crystallinity of the polymer electrolytes using Bruker (D8 Advance) diffractometerand Perkin-Elmer (Paragon 500 grating) IR spectrophotometer respectively. Thermal stability of the film wasalso characterized by TG/DTA at a heating rate of 10C per minute from room temperature. The electricalconductivity of polymer complexes was measured from impedance plots at different temperatures usingKeithley 3330 LCZ meter. The impedance measurement was recorded in the frequency range 40Hz-100 KHzwith signal amplitude of 10mV.
Effects of addition of BaTiO3 nano particles on the conductivity of PVdF/PMMA based polymer blendelectrolyteswww.ijeijournal.com Page | 50III. Results and Discussion3.1 X-ray diffractionX-ray diffraction patterns of pure PVdF, PMMA, LiBF4 and PVdF(17.5)- PMMA(7.5)- PC(67)-LiBF4(8) with X % of BaTiO3 (where X= 0,5,10,15,20) in the total polymer weight are shown in the figure 1.The nano sized BaTiO3 dispersed emulsion can penetrate the space between the polymer chains andconsequently, the homogeneously dispersed ceramic filler in the matrix prevents or retards crystallization of thepolymers due to its large surface area. The intensity of the peaks abruptly decreases in the compositeelectrolytes. No peaks have appeared corresponding to the salt in the complexes, which confirms theamorphicity of the electrolytes. These observations illustrate that the polymer electrolytes have turned to anamorphous phase.3.2 FT-IR analysisFT-IR studies were carried out using FTIR ABB BOMEN MB104 IR spectrophotometer at 0.9 cm-1resolution. The characteristic vibrational frequencies at 3010 and 2951 cm-1are assigned to O–CH2 asymmetricstretching and CH3 asymmetric stretching of PMMA, which are displaced to 2995 and 2947 cm-1in thecomplexes. The vibrational peaks appearing at 1389 and 1280 cm-1are assigned to O–CH3 deformation and C–O stretching of PMMA. They are shifted to 1392 and 1276 cm-1in the complexes. The C=O stretching, CH2scissoring, twisting, wagging modes of PMMA at 1736, 1483, 1173 and 947 cm-1are found to be absent in thecomplexes.The vibrational bands at 1263 and 1186 cm-1are ascribed to the stretching frequencies of C–F and CF2,respectively, in pure PVdF. Also the peaks at 1070 and 533 cm-1are ascribed to symmetric C–C stretching andCF2 bending vibrations of pure PVdF, respectively. In the blended polymer complexes, the vibrational bandobserved at 875–870 cm-1is ascribed to the combinations of symmetric C–C stretching and skeletal CF–CH–CHbending of PVdF. The peaks observed at 1268 cm-1is ascribed to C–F stretching vibrations of PVdF,respectively.It is also found that some of the peaks disappear in the complexes such as (976, 1185, 1724, 2645, 3435cm-1). In addition to this, few new peaks are observed at (489, 881, 1800, 2085 cm-1) in the polymer complexes.The above analysis confirms the complex formation.3.3 Conductivity studiesFigure 3 shows the complex impedance plot of PVdF(17.5)- PMMA(7.5)- PC(67)- LiBF4(8) with 15wt % of BaTiO3 of the total polymer weight at various temperatures. This plot shows linear spikes. Thedisappearance of the high frequency semicircular portion in the polymer complex impedance plot indicates thatthe current carriers are ions and the total conductivity is the result of ion conduction. The bulk resistance of theelectrolyte was measured by extrapolating an intercept of this plot on the real axis. The electrical conductivity ofthe electrolyte was calculated for the known values of bulk resistance (Rb), area (A) and the thickness (l) of thefilm using the formula σ = l/RbA.It has been seen that the addition of inorganic fillers leads to an increase in the ambient temperatureconductivity upto 15 wt% of BaTiO3 in the total polymer weight and then the ionic conductivity decreases dueto higher concentration of ceramic fillers. Indeed, one may surmise that the presence of high dispersed particlesin the polymer matrix may affect the crystallization rate by preventing the agglomeration of the polymer chains.Further, the particle size and content of the ceramic additive appear to be a critical factor. It is also seen that areasonably high concentration of the filler is also necessary to affect the recrystallization rate of the polymerhost.The temperature dependence of the ionic conductivity of PVdF(17.5)- PMMA(7.5)- PC(67)- LiBF4(8)-X% of BaTiO3 (where X= 0,5,10,15,20) in the total polymer electrolyte is shown in the figure 4. From the plot ithas been observed that as temperature increases the conductivity values also increase for all the compositions.The non-linearity in Arrhenius plots indicates that ion transport in polymer electrolytes is dependent on polymersegmental motion. The curvature behaviour of the plots suggests that the data can be better described by theVogel–Tamman–Fulcher (VTF) relation, which described the transport properties in a viscous matrix. Itsupports the idea that the ion moves through the plasticizer-rich phase.3.4 Thermal analysisFigure 5 shows the TG/DTA traces of PVdF (17.5)-PMMA (7.5)-PC (67)-LiBF4 (8)- BaTiO3 (15 wt%)polymer composite which shows maximum conductivity value. An endothermic peak was observed at 35C andcorresponding about 2% of weight loss is attributed to the presence of moisture in the samples. The film startsdecomposing at 251C followed by an endothermic peak, which indicates that the film is stable up to 251C.
Effects of addition of BaTiO3 nano particles on the conductivity of PVdF/PMMA based polymer blendelectrolyteswww.ijeijournal.com Page | 51The DTA trace shows an endothermic peak around 360C, which corresponds to the melting point of PMMApolymer host.It is clear from these observations, that the PMMA based hybrid polymer electrolytes, which containLiClO4 as salt can be operated up to 251C.IV. ConclusionThe salt-in-polymer electrolytes prepared from the PVdF/PMMA show a strong enhancement of theionic conductivity by the addition of BaTiO3 nanoparticles. The ionic conductivity of the resulting compositepolymer electrolyte is better than the blend polymer electrolyte. The temperature dependent ionic conductivityplot of the composite films seems to obey the VTF relation.Reference Tigelaar, D.M.; Meador, M.A.B.; Bennett, W.R. Macromolecules, 2007, 40, pp. 4159. Liu, Y.; Lee, J.Y.; Kang, E.T.; Wang, P.; Tan, K.L. React. Funct. Polym., 2001, 47, pp. 201. Fenton, D.E.; Parker, J.M.; Wright, P.V. Polymer, 1973, 14, pp. 589. Croce, F.; Appetecchi, G.B.; Persi, L.; Scrosati, B. Nature, 1998, 394, pp. 456. Dias, F.B.; Plomp, L.; Veldhuis, J.P.J. J. Power Sources, 2000, 88, pp. 169. Xi, J.; Qiu, X.; Cui, M.; Tang, X.; Zhu, W.; Chen, L. J. Power Sources, 2006,156, pp. 581. Kao, H.M.; Chen, C.L. Angew. Chem. Int. Ed., 2004, 43, pp. 980. Croce, F.; Cuini, R.; Matinelli, A.; Persi, L.; Ronci, F.; Scrosati, B. J. Phys. Chem. B, 1999, 103, pp. 10632. Chung, S.H.; Wang, Y.; Persi, L.; Croce, F.; Greenbaum, S.G.; Scrosati, B.; Plichta, E. J. Power Sources, 2001, 97–98,pp.644. Jayathilaka, P.A.R.D.; Dissanayake, M.A.K.L.; Albinsson, I.; Mellander, B.E. Electrochim. Acta, 2002, 47, pp. 3257. Marcinek, M.; Bac, A.; Lipka, P.; Zalewska, A.; Zukowska, G.; Borkowska, R.; Wieczorek, W. J. Phys. Chem. B, 2000, 104, pp.11088.Figure 1. X-ray diffraction patterns of (a) Pure PVdF (b) Pure PMMA (c) BaTiO3(d) PVdF (17.5)-PMMA (7.5)-LiBF4 (8)-PC (67)-BaTiO3 (0)(e) PVdF (17.5)-PMMA (7.5)-LiBF4 (8)-PC (67)-BaTiO3 (5)(f) PVdF (17.5)-PMMA (7.5)-LiBF4 (8)-PC (67)-BaTiO3 (10)(g) PVdF(17.5)-PMMA(7.5)-LiBF4(8)-PC(67)-BaTiO3(15)(h) PVdF(17.5)-PMMA(7.5)-LiBF4(8)-PC(67)-BaTiO3(20)
Effects of addition of BaTiO3 nano particles on the conductivity of PVdF/PMMA based polymer blendelectrolyteswww.ijeijournal.com Page | 52Figure 2. FTIR Spectra of (a) Pure PVdF (b) Pure PMMA (c) LiBF4(d) PVdF (17.5)-PMMA (7.5)-LiBF4 (8)-PC (67)-BaTiO3(0)(e) PVdF (17.5)-PMMA (7.5)-LiBF4 (8)-PC (67)-BaTiO3(5)(f) PVdF (17.5)-PMMA (7.5)-LiBF4 (8)-PC (67)-BaTiO3(10)(g) PVdF(17.5)-PMMA(7.5)-LiBF4(8)-PC(67)-BaTiO3(15)(h) PVdF(17.5)-PMMA(7.5)-LiBF4(8)-PC(67)-BaTiO3(20)Figure 3. Impedance diagram for PVdF(17.5)-PMMA(7.5)-LiBF4(8) -PC(67)-BaTiO3(10) wt% at varioustemperatures.
Effects of addition of BaTiO3 nano particles on the conductivity of PVdF/PMMA based polymer blendelectrolyteswww.ijeijournal.com Page | 53Figure 4. Arrhenius plot of PVdF(17.5)-PMMA(7.5)-LiBF4(8)-PC(67)- BaTiO3(X wt %) (where X= 0, 5, 10, 15,20) composites.Figure 5. TG/DTA curves of PVdF(17.5)-PMMA(7.5)-LiBF4(8)-PC(67)- BaTiO3(15 wt %) composite.Table 1Ionic conductivity values for PVdF (17.5)-PMMA (7.5) -PC (67) - LiBF4 (8) – BaTiO3(X wt %) (where X= 0, 5,10, 15, 20) systemFilm BaTiO3 ratio Ionic conductivity x 10-3S cm-1301K 311K 321K 331K 341KV1 0 0.854 0.988 1.101 1.256 1.372V2 5 1.113 1.283 1.401 1.493 1.591V3 10 1.335 1.463 1.531 1.611 1.726V4 15 1.297 1.303 1.412 1.528 1.679V5 20 1.064 1.256 1.397 1.456 1.512